#------------------------------------------------------------------------------
#$Date: 2022-10-03 17:40:12 +0300 (Mon, 03 Oct 2022) $
#$Revision: 278324 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/00/20/2002025.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2002025
loop_
_publ_author_name
'Foulon, J.-D.'
'Tijani, N.'
'Durand, J.'
'Rafiq, M.'
'Cot, L.'
_publ_section_title
;
 Structure de Ln₂(PO₃H)₃.H₂O (Ln = Pr, Nd)
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              1
_journal_page_last               4
_journal_paper_doi               10.1107/S0108270192004050
_journal_volume                  49
_journal_year                    1993
_chemical_formula_sum            'H5 O10 P3 Pr2'
_chemical_formula_weight         539.8
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.980(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.620(2)
_cell_length_b                   8.0050(10)
_cell_length_c                   13.119(2)
_cell_volume                     949.5(3)
_diffrn_radiation_type           Mo
_diffrn_radiation_wavelength     0.71073
_exptl_absorpt_coefficient_mu    10.68
_exptl_crystal_density_diffrn    3.754
_exptl_crystal_density_meas      3.720(10)
_exptl_crystal_F_000             992
_cod_data_source_file            du0341.cif
_cod_data_source_block           du0341_structure_1_of_2
_cod_depositor_comments
;
 Adding the _atom_site_type_symbol data item.

 Antanas Vaitkus,
 2017-01-15
;
_cod_original_cell_volume        955.4(3)
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               2002025
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x+1/2,y+1/2,-z+1/2
3 -x,-y,-z
4 x+1/2,-y+1/2,z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
Pr(1) Pr .44886(4) .57770(5) .26809(3) .0080(2)
Pr(2) Pr .87142(4) .71232(5) .46211(3) .0070(2)
P(1) P .1690(2) .6966(2) .4015(2) .0100(10)
P(2) P .6091(2) .7514(2) .5543(2) .0090(10)
P(3) P .7138(2) .6153(2) .1719(2) .0080(10)
O(11) O .0500(7) .8295(7) .3575(5) .015(3)
O(12) O .0982(7) .5639(7) .4542(5) .016(3)
O(13) O .2350(6) .6209(7) .3225(5) .014(3)
O(21) O .6092(6) .6564(8) .4525(4) .015(3)
O(22) O .7680(7) .8120(8) .6061(5) .017(3)
O(23) O .5462(7) .6575(7) .6286(5) .016(3)
O(31) O .5549(6) .6718(7) .1147(5) .015(3)
O(32) O .7270(6) .5885(7) .2905(5) .014(3)
O(33) O .7554(6) .4627(7) .1201(5) .015(3)
HW O .4547(8) .8860(8) .2951(5) .027(4)
H(1) H .2834 .7534 .4847 .030
H(2) H .5097 .8794 .5115 .030
H(3) H .8220 .7306 .1904 .030
H(W1) H .3880 .9952 .2943 .050
H(W2) H .5603 .9354 .2984 .050
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
O(11) P(1) O(12) 105.2(3)
O(11) P(1) O(13) 116.8(3)
O(12) P(1) O(13) 112.2(3)
O(11) P(1) H(1) 112.5
O(12) P(1) H(1) 103.4
O(13) P(1) H(1) 106.0
O(21) P(2) O(22) 105.0(3)
O(21) P(2) O(23) 115.4(3)
O(22) P(2) O(23) 115.0(3)
O(21) P(2) H(2) 101.3
O(22) P(2) H(2) 115.0
O(23) P(2) H(2) 114.5
O(31) P(3) O(32) 106.1(3)
O(31) P(3) O(33) 112.6(3)
O(32) P(3) O(33) 113.3(3)
O(31) P(3) H(3) 118.2
O(32) P(3) H(3) 96.2
O(33) P(3) H(3) 109.3
Pr(1) HW H(W1) 144.4
Pr(1) H H(W2) 110.2
H(W1) H H(W2) 104.6
HW H(W1) O(13) 130.5
HW H(W2) O(33) 145.1
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
P(1) O(11) 1.531(6)
P(1) O(12) 1.543(6)
P(1) O(13) 1.506(6)
P(1) H(1) 1.35
P(2) O(21) 1.538(6)
P(2) O(22) 1.535(6)
P(2) O(23) 1.505(6)
P(2) H(2) 1.35
P(3) O(31) 1.535(6)
P(3) O(32) 1.535(6)
P(3) O(33) 1.514(6)
P(3) H(3) 1.35
Pr(1) O(11) 2.583(6)
Pr(1) O(13) 2.413(7)
Pr(1) O(21) 2.490(6)
Pr(1) O(22) 2.433(6)
Pr(1) O(23) 2.311(6)
Pr(1) O(31) 2.645(6)
Pr(1) O(32) 2.597(6)
Pr(2) O(11) 2.693(6)
Pr(2) O(12) 2.516(6)
Pr(2) O(12) 2.443(6)
Pr(2) O(21) 2.524(6)
Pr(2) O(22) 2.534(6)
Pr(2) O(31) 2.385(6)
Pr(2) O(32) 2.439(6)
Pr(2) O(33) 2.411(6)
